- About this Journal ·
- Abstracting and Indexing ·
- Aims and Scope ·
- Annual Issues ·
- Article Processing Charges ·
- Author Guidelines ·
- Bibliographic Information ·
- Citations to this Journal ·
- Contact Information ·
- Editorial Board ·
- Editorial Workflow ·
- Free eTOC Alerts ·
- Publication Ethics ·
- Recently Accepted Articles ·
- Reviewers Acknowledgment ·
- Submit a Manuscript ·
- Subscription Information ·
- Table of Contents
Journal of Nanomaterials
Volume 2014 (2014), Article ID 539295, 5 pages
Observation and Characterization of Fragile Organometallic Molecules Encapsulated in Single-Wall Carbon Nanotubes
1Department of Chemistry, Nagoya University, Nagoya 464-8602, Japan
2Department of Chemistry, The University of Tokyo, Tokyo 113-0033, Japan
3Nanotube Research Center, National Institute of Advanced Industrial Science and Technology, Tsukuba 305-8565, Japan
4Department of Information and Biological Science, Nagoya City University, Nagoya 467-8501, Japan
5Division of Physics, Faculty of Pure and Applied Sciences, University of Tsukuba, 1-1-1 Tennodai, Tsukuba, Ibaraki 305-8571, Japan
6Japan Synchrotron Radiation Research Institute, Hyogo 679-5198, Japan
Received 26 February 2014; Accepted 21 April 2014; Published 9 June 2014
Academic Editor: Keita Kobayashi
Copyright © 2014 Daisuke Ogawa et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.
Thermally fragile tris(-cyclopentadienyl)erbium (ErCp3) molecules are encapsulated in single-wall carbon nanotubes (SWCNTs) with high yield. We realized the encapsulation of ErCp3 with high filling ratio by using high quality SWCNTs at an optimized temperature under higher vacuum. Structure determination based on high-resolution transmission electron microscope observations together with the image simulations reveals the presence of almost free rotation of each ErCp3 molecule in SWCNTs. The encapsulation is also confirmed by X-ray diffraction. Trivalent character of Er ions (i.e., Er3+) is confirmed by X-ray absorption spectrum.
Nanowires with a few atoms in diameter show completely different properties from those of the three-dimensional bulk materials [1–11]. However, in general, those ultimately thin nanowires are unstable under atmospheric conditions and they are therefore quite difficult to realize.
In 1998, it was found that single-wall carbon nanotubes (SWCNTs) are able to encapsulate C60 fullerenes in their inner hollow space . Since the discovery, various materials have been encapsulated in SWCNTs, which has produced a wide variety of low-dimensional hybrid nanomaterials; SWCNTs have provided ideal nanospace and protective walls for encapsulated materials [13–17]. In addition to their specific structure, these newly formed hybrid nanomaterials have shown interesting properties [18–20].
The encapsulation of organometallic complex molecules, such as Co(C5H5)2  and Fe(C5H5)2 [22–25], in the SWCNTs has attracted wide attention due to an expected control of SWCNT’s electronic properties through charge transfer between encapsulates and SWCNT. Furthermore, organometallics can act as a precursor to form metal atomic wires in SWCNTs via the so-called nanotemplate reaction, which may lead to the formation of novel metal atomic wires.
Encapsulation of organometallics in SWCNTs, however, has so far been difficult, mainly because of the fact that, under atmospheric condition or at high temperature, such materials normally decompose during the encapsulation process. Here, we have focused on the development of a versatile method to encapsulate fragile organometallic complexes in SWCNTs. To confirm the encapsulation, we have employed a structure determination procedure that is based on high-resolution transmission electron microscope (HR-TEM) observations and HR-TEM image simulation by the multislice method .
SWCNTs were synthesized by the so-called extended direct injection pyrolytic synthesis (e-DIPS) . As-produced e-DIPS SWCNTs (a-CNTs) were annealed at 1200°C in vacuum (~10−5 Pa) for 14 hours in order to remove remaining Fe catalyst nanoparticles and amorphous carbon impurities . Before the encapsulation reaction, the purified e-DIPS SWCNTs (p-CNTs) were heated under dry air flow at 600°C for 30 min in order to open the endcap of SWCNTs.
ErCp3 is an air- and moisture-sensitive material and decomposes easily upon exposure to the atmosphere . ErCp3 was thus carefully handled and purified by sublimation at 200°C under high vacuum (~10−4 Pa)  and was kept in an anaerobic glove box. In the following experiments, all the sample preparation was performed using the purified ErCp3 under anaerobic condition to avoid any undesired degradation of ErCp3 during the preparation. Open-ended p-CNTs (o-CNTs) were vacuum sealed (~10−4 Pa) in a Pyrex tube with the purified ErCp3, and the sealed Pyrex tube was heated at 250°C for 72 hours. At this temperature and pressure, ErCp3 was sublimed and encapsulated in the hollow space of the SWCNTs. The as-prepared ErCp3@o-CNTs were washed with anhydrous tetrahydrofuran in order to remove any ErCp3 molecules physically adsorbed on the outer surface of the SWCNTs. The final products were dried at 80°C for 12 hours. As a control experiment, we also prepared a sample, ErCp3@p-CNTs, by performing the encapsulation process of ErCp3 on p-CNTs.
3. Results and Discussion
Figure 1 shows a thermal gravimetric analysis (TGA) trace of a-CNTs and p-CNTs. Two shoulders were clearly seen at around 400°C and 600°C on the TGA curve of a-CNTs. The former and the latter shoulders correspond to the oxidation of amorphous carbon and the oxidation of SWCNTs and graphite, respectively. In contrast, only one sharp drop at 500°C and a smaller amount of residual material (3.84 wt.%) were observed in the TGA curve of p-CNTs, which indicates higher purity of p-CNTs than that of a-CNTs.
Figures 2(a) and 2(b) are HR-TEM images of a-CNTs and p-CNTs, respectively. As seen in Figure 2(a), dark contrasts of Fe catalyst nanoparticles and amorphous impurity attached outer surface of SWCNTs are clearly observed. The amount of Fe catalyst nanoparticles and amorphous impurity greatly decreases after purification, as shown in Figure 2(b). In Figures S1(a) and (b) (see Figures S1(a) and S1(b) in Supplementary Material available online at http://dx.doi.org/10.1155/2014/539295), the corresponding energy dispersive X-ray (EDX) spectra are shown. Obtained spectra clearly show that the amount of residual Fe had been greatly reduced by purification. These HR-TEM images are consistent with the TGA results.
Figures 3(a) and 3(b) show HR-TEM images of ErCp3@o-CNTs having different tube diameters. As seen in Figure 3(a), dot-like contrasts align in one-dimensional fashion at intervals of 0.94 nm inside SWCNTs whose diameter is 1.30 nm. The observed interval of 0.94 nm is almost the same with the molecular size of the ErCp3 molecule; the molecular size was estimated considering van der Waals radius of constituent atoms. Moreover, the difference between the diameter of SWCNTs (i.e., 1.30 nm) and the intervals of dot-like contrasts (i.e., 0.94 nm) observed is nearly equal to the van der Waals radii of the inner wall of SWCNTs (~0.34 nm) [30, 31].
When the diameter of SWCNTs is larger than 1.30 nm, ErCp3 molecules aggregate to form clusters (Figure 3(b)). An EDX spectrum observed in the same area shows strong peaks that can be attributed to Er , , and (Figure S1(c)). The dark spots were not observed in o-CNTs prior to the ErCp3 encapsulation, and no EDX peaks from Er atoms were observed. Therefore, we conclude that observed contrasts arise from encapsulated ErCp3 molecules forming one-dimensional regular array in hollow space of SWCNTs. The estimated filling ratio from the HR-TEM images is ca. 30% or more, which is substantially higher than that previously reported for organometallic complexes molecules encapsulated in SWCNTs [21, 22].
To confirm the high filling ratio of ErCp3 in o-CNTs, we have measured X-ray diffraction (XRD) patterns. Figures S2(a) and (b) show the XRD patterns of o-CNTs, ErCp3@o-CNTs, p-CNTs, and ErCp3@p-CNTs. As shown in Figures S2(a) and (b), the number of diffraction peaks is limited, so that it is difficult to determine precise filling ratio by pattern fitting. Filling of ErCp3 molecules, however, can be confirmed by changes in intensity of (10) peak. As clearly seen in Figure S2(a), the intensity of (10) peak of ErCp3@o-CNTs is much smaller than that of o-CNTs. This is a clear indication that the inner space of o-CNTs is filled with guest materials (i.e., ErCp3) [14, 32, 33].
The intensity of (10) peak of ErCp3@p-CNTs is comparable to that of p-CNTs, suggesting that the observed intensity drop in ErCp3@o-CNTs can be attributed to encapsulation of ErCp3 molecules (Figure S2(b)). The high filling ratio is caused by (1) purification and anaerobic handling of ErCp3, (2) an improved preparation method of o-CNTs (i.e., high quality, proper diameter, and optimized cap-opening conditions), and (3) performing the encapsulation reaction under high vacuum at optimized conditions.
Based on the observed HR-TEM images of ErCp3@SWCNT, we have constructed a structure model. Image simulations by the multislice method (at a defocus of 600, 650, 700, 750, and 800 nm) have been carried out based on the structure model constructed. To attain satisfactory agreements between the observed and simulated HR-TEM images, we have superimposed simulated HR-TEM images of ErCp3@SWCNT with different molecular orientations, in which simulated images based on fixed molecular orientations do not match with the observed images.
As illustrated in inset of Figure 3(a), the final simulated HR-TEM image well reproduces both the observed dark ellipsoids and their intensities. Hence, encapsulated ErCp3 molecules may be rotating much faster than the time scale of HR-TEM observation (the typical exposure time is several seconds). This suggests that the interaction between encapsulated ErCp3 and SWCNTs should fairly be weak. Since the ionization energy of ErCp3 (7~8 eV) is much larger than the threshold under which charge transfer interaction between SWCNTs occurs ; the interaction between ErCp3 and SWCNTs should not be significant. Here the ionization energy of ErCp3 was estimated from the ionization energy of other molecules, that is, LaCp3 (7.9 eV), PrCp3 (7.68 eV), and TmCp3 (7.43 eV), respectively .
To further investigate the electronic structure of ErCp3, X-ray absorption spectrum (XAS) measurements at the Er absorption edge were performed, which indicates trivalency of Er ions (i.e., Er3+) (Figure 4). The spectrum is almost identical to that of Er2O3, suggesting that encapsulated ErCp3 molecules do not transform into any clusters or aggregates as such. SWCNTs act only as a template that restricts the space where ErCp3 molecules are encapsulated. The restricted space of SWCNTs is, therefore, well suited to stabilize unstable metal-containing complexes and to create low-dimensional alignment of various metal complexes including unstable organometallics.
We have successfully fabricated novel low-dimensional crystalline ErCp3 nanowires encapsulated in SWCNTs with filling yield of ~30% and characterized their structural properties. Encapsulation reactions carried out under high temperature and high vacuum conditions using high quality SWCNTs are necessary in order to obtain ErCp3@SWCNTs. A structure determination method based on the simulated annealing method and HR-TEM image simulation has been shown to be useful in characterizing the crystal structure of metal complex nanowires formed in SWCNTs. The present study may lead to future fabrication of various low-dimensional metal complexes in SWCNTs in high yield.
Conflict of Interests
The authors declare that there is no conflict of interests regarding the publication of this paper.
Hisanori Shinohara acknowledges the Grant-in-Aid for Scientific Research (S) (no. 22225001) of MEXT, Japan, for the partial support of the present study. The XRD experiments were performed at BL02B2 and XAS experiments were performed at BL25SU in SPring-8 with the approval of JASRT.
- Y. Wu, J. Xiang, C. Yang, W. Lu, and C. M. Lieber, “Single-crystal metallic nanowires and metal/semiconductor nanowire heterostructures,” Nature, vol. 430, no. 6995, pp. 61–65, 2004.
- Y. Kondo and K. Takayanagi, “Synthesis and characterization of helical multi-shell gold nanowires,” Science, vol. 289, no. 5479, pp. 606–608, 2000.
- R. He and P. Yang, “Giant piezoresistance effect in silicon nanowires,” Nature Nanotechnology, vol. 1, no. 1, pp. 42–46, 2006.
- J. Xiang, W. Lu, Y. Hu, Y. Wu, H. Yan, and C. M. Lieber, “Ge/Si nanowire heterostructures as high-performance field-effect transistors,” Nature, vol. 441, no. 7092, pp. 489–493, 2006.
- B. R. McNamara, P. E. J. Nulsen, M. W. Wise et al., “The heating of gas in a galaxy cluster by X-ray cavities and large-scale shock fronts,” Nature, vol. 433, no. 7021, pp. 45–47, 2005.
- T. Yoshie, A. Scherer, J. Hendrickson et al., “Vacuum Rabi splitting with a single quantum dot in a photonic crystal nanocavity,” Nature, vol. 432, no. 7014, pp. 200–203, 2004.
- L. Mohaddes-Ardabili, H. Zheng, S. B. Ogale et al., “Self-assembled single-crystal ferromagnetic iron nanowires formed by decomposition,” Nature Materials, vol. 3, no. 8, pp. 533–538, 2004.
- D. D. D. Ma, C. S. Lee, F. C. K. Au, S. Y. Tong, and S. T. Lee, “Small-diameter silicon nanowire surfaces,” Science, vol. 299, no. 5614, pp. 1874–1877, 2003.
- B. H. Hong, S. C. Bae, C.-W. Lee, S. Jeong, and K. S. Kim, “Ultrathin single-crystalline silver nanowire arrays formed in an ambient solution phase,” Science, vol. 294, no. 5541, pp. 348–351, 2001.
- C. Zeng, P. R. C. Kent, T.-H. Kim, A.-P. Li, and H. H. Weitering, “Charge-order fluctuations in one-dimensional silicides,” Nature Materials, vol. 7, no. 7, pp. 539–542, 2008.
- H. Ohnishi, Y. Kondo, and K. Takayanagi, “Quantized conductance through individual rows of suspended gold atoms,” Nature, vol. 395, no. 6704, pp. 780–783, 1998.
- B. W. Smith, M. Monthioux, and D. E. Luzzi, “Encapsulated C60 in carbon nanotubes,” Nature, vol. 396, no. 6709, pp. 323–324, 1998.
- J. Lee, H. Kim, S. J. Kahng et al., “Bandgap modulation of carbon nanotubes by encapsulated metallofullerenes,” Nature, vol. 415, no. 6875, pp. 1005–1008, 2002.
- T. Takenobu, T. Takano, M. Shiraishi et al., “Stable and controlled amphoteric doping by encapsulation of organic molecules inside carbon nanotubes,” Nature Materials, vol. 2, no. 10, pp. 683–688, 2003.
- E. Philp, J. Sloan, A. I. Kirkland et al., “An encapsulated helical one-dimensional cobalt iodide nanostructure,” Nature Materials, vol. 2, no. 12, pp. 788–791, 2003.
- M. A. Loi, J. Gao, F. Cordella et al., “Encapsulation of conjugated oligomers in single-walled carbon nanotubes: towards nanohybrids for photonic devices,” Advanced Materials, vol. 22, no. 14, pp. 1635–1639, 2010.
- T. Iwamoto, Y. Watanabe, T. Sadahiro, T. Haino, and S. Yamago, “Size-selective encapsulation of C60 by cycloparaphenylene: formation of the shortest fullerene-peapod,” Angewandte Chemie—International Edition, vol. 50, no. 36, pp. 8342–8344, 2011.
- J. Vavro, J. M. Kikkawa, and J. E. Fischer, “Metal-insulator transition in doped single-wall carbon nanotubes,” Physical Review B, vol. 71, no. 15, Article ID 155410, 11 pages, 2005.
- A. Javey, R. Tu, D. B. Farmer, J. Guo, R. G. Gordon, and H. J. Dai, “High performance n-type carbon nanotube field-effect transistors with chemically doped contacts,” Nano Letters, vol. 5, no. 2, pp. 345–348, 2005.
- E. Gaufres, N. Y.-W. Tang, F. Lapointe et al., “Giant Raman scattering from J-aggregated dyes inside carbon nanotubes for multispectral imaging,” Nature Photonics, vol. 8, no. 1, pp. 72–78, 2013.
- L. J. Li, A. N. Khlobystov, J. G. Wiltshire, G. A. D. Briggs, and R. J. Nicholas, “Diameter-selective encapsulation of metallocenes in single-walled carbon nanotubes,” Nature Materials, vol. 4, no. 6, pp. 481–485, 2005.
- Y. F. Li, R. Hatakeyama, T. Kaneko, and T. Okada, “Nano sized magnetic particles with diameters less than 1 nm encapsulated in single-walled carbon nanotubes,” Japanese Journal of Applied Physics, vol. 45, no. 12–16, pp. L428–L431, 2006.
- Y. F. Li, T. Kaneko, T. Ogawa, M. Takahashi, and R. Hatakeyama, “Novel properties of single-walled carbon nanotubes with encapsulated magnetic atoms,” Japanese Journal of Applied Physics, vol. 47, no. 4, pp. 2048–2055, 2008.
- H. Shiozawa, T. Pichler, R. Pfeiffer, H. Kuzmany, and H. Kataura, “Ferrocene encapsulated in single-wall carbon nanotubes: a precursor to secondary tubes,” Physica Status Solidi B, vol. 244, no. 11, pp. 4102–4105, 2007.
- M. Sauer, H. Shiozawa, P. Ayala et al., “Environmental stability of ferrocene filled in purely metallic single-walled carbon nanotubes,” Physica Status Solidi B, vol. 250, no. 12, pp. 2599–2604, 2013.
- S. Kirkpatrick, C. D. Gelatt Jr., and M. P. Vecchi, “Optimization by simulated annealing,” Science, vol. 220, no. 4598, pp. 671–680, 1983.
- T. Saito, W. C. Xu, S. Ohshima, H. Ago, M. Yumura, and S. Iijima, “Supramolecular catalysts for the gas-phase synthesis of single-walled carbon nanotubes,” Journal of Physical Chemistry B, vol. 110, no. 12, pp. 5849–5853, 2006.
- R. Kitaura, D. Ogawa, K. Kobayashi et al., “High yield synthesis and characterization of the structural and magnetic properties of crystalline ErCl3 nanowires in single-walled carbon nanotube templates,” Nano Research, vol. 1, no. 2, pp. 152–157, 2008.
- J. M. Birmingham and G. Wilkinson, “The cyclopentadienides of scandium, yttrium and some rare earth elements,” Journal of the American Chemical Society, vol. 78, no. 1, pp. 42–44, 1956.
- A. Bondi, “Van der Waals volumes and radii,” Journal of Physical Chemistry, vol. 68, no. 3, pp. 441–451, 1964.
- S. Bandow, M. Takizawa, H. Kato, T. Okazaki, H. Shinohara, and S. Iijima, “Smallest limit of tube diameters for encasing of particular fullerenes determined by radial breathing mode Raman scattering,” Chemical Physics Letters, vol. 347, no. 1–3, pp. 23–28, 2001.
- Y. Maniwa, Y. Kumazawa, Y. Saito et al., “Anomaly of X-ray diffraction profile in single-walled carbon nanotubes,” Japanese Journal of Applied Physics, vol. 38, no. 6, pp. L668–L670, 1999.
- Y. Maniwa, H. Kataura, M. Abe et al., “Phase transition in confined water inside carbon nanotubes,” Journal of the Physical Society of Japan, vol. 71, no. 12, pp. 2863–2866, 2002.
- S. G. Lias, J. E. Bartmess, J. F. Liebman, J. L. Holmes, R. D. Levin, and W. G. Mallard, Gas Phase Ion and Neutral Thermochemistry, Journal of Physical and Chemical Reference Data, vol. 17, Supplement, no. 1, The American Chemical Society and the American Institute of Physics for the National Bureau of Standards, New York, NY, USA, 1988.